* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project

# Download Piezo-Fundamentals.pdf

Survey

Document related concepts

History of metamaterials wikipedia , lookup

Shape-memory alloy wikipedia , lookup

Scanning SQUID microscope wikipedia , lookup

Electricity wikipedia , lookup

Strengthening mechanisms of materials wikipedia , lookup

Hall effect wikipedia , lookup

Viscoplasticity wikipedia , lookup

Paleostress inversion wikipedia , lookup

Fatigue (material) wikipedia , lookup

Hooke's law wikipedia , lookup

Deformation (mechanics) wikipedia , lookup

Work hardening wikipedia , lookup

Multiferroics wikipedia , lookup

Viscoelasticity wikipedia , lookup

Energy harvesting wikipedia , lookup

Transcript

2 Fundamentals of Piezoelectricity 2.1 Introduction This chapter is concerned with piezoelectric materials and their properties. We begin the chapter with a brief overview of some historical milestones, such as the discovery of the piezoelectric eﬀect, the invention of piezoelectric ceramic materials, and commercial and military utilization of the technology. We will review important properties of piezoelectric ceramic materials and will then proceed to a detailed introduction of the piezoelectric constitutive equations. The main assumption made in this chapter is that transducers made from piezoelectric materials are linear devices whose properties are governed by a set of tensor equations. This is consistent with the IEEE standards of piezoelectricity [154]. We will explain the physical meaning of parameters which describe the piezoelectric property, and will clarify how these parameters can be obtained from a set of simple experiments. In this book, piezoelectric transducers are used as sensors and actuators in vibration control systems. For this purpose, transducers are bonded to a ﬂexible structure and utilized as either a sensors to monitor structural vibrations, or as actuators to add damping to the structure. To develop model-based controllers capable of adding suﬃcient damping to a structure using piezoelectric actuators and sensors it is vital to have models that describe the dynamics of such systems with suﬃcient precision. We will explain how the dynamics of a ﬂexible structure with incorporated piezoelectric sensors and actuators can be derived starting from physical principles. In particular, we will emphasize the structure of the models that are obtained from such an exercise. Knowledge of the model structure is crucial to the development of precise models based on measured frequency domain data. This will constitute our main approach to obtaining models of systems studied throughout this book. 10 2 Fundamentals of Piezoelectricity 2.2 History of Piezoelectricity The ﬁrst scientiﬁc publication describing the phenomenon, later termed as piezoelectricity, appeared in 1880 [48]. It was co-authored by Pierre and Jacques Curie, who were conducting a variety of experiments on a range of crystals at the time. In those experiments, they cataloged a number of crystals, such as tourmaline, quartz, topaz, cane sugar and Rochelle salt that displayed surface charges when they were mechanically stressed. In the scientiﬁc community of the time, this observation was considered as a signiﬁcant discovery, and the term “piezoelectricity” was coined to express this eﬀect. The word “piezo” is a Greek word which means “to press”. Therefore, piezoelectricity means electricity generated from pressure - a very logical name. This terminology helped distinguish piezoelectricity from the other related phenomena of interest at the time; namely, contact electricity1 and pyroelectricity2 . The discovery of the direct piezoelectric eﬀect is, therefore, credited to the Curie brothers. They did not, however, discover the converse piezoelectric eﬀect. Rather, it was mathematically predicted from fundamental laws of thermodynamics by Lippmann [118] in 1881. Having said this, the Curies are recognized for experimental conﬁrmation of the converse eﬀect following Lippmann’s work. The discovery of piezoelectricity generated signiﬁcant interest within the European scientiﬁc community. Subsequently, roughly within 30 years of its discovery, and prior to World War I, the study of piezoelectricity was viewed as a credible scientiﬁc activity. Issues such as reversible exchange of electrical and mechanical energy, asymmetric nature of piezoelectric crystals, and the use of thermodynamics in describing various aspects of piezoelectricity were studied in this period. The ﬁrst serious application for piezoelectric materials appeared during World War I. This work is credited to Paul Langevin and his co-workers in France, who built an ultrasonic submarine detector. The transducer they built was made of a mosaic of thin quartz crystals that was glued between two steel plates in a way that the composite system had a resonance frequency of 50 KHz. The device was used to transmit a high-frequency chirp signal into the water and to measure the depth by timing the return echo. Their invention, however, was not perfected until the end of the war. Following their successful use in sonar transducers, and between the two World Wars, piezoelectric crystals were employed in many applications. Quartz crystals were used in the development of frequency stabilizers for vacuum-tube oscillators. Ultrasonic transducers manufactured from piezoelectric crystals were used for measurement of material properties. Many of the classic piezoelectric applications that we are familiar with, applications such 1 2 Static electricity generated by friction Electricity generated from crystals, when heated 2.3 Piezoelectric Ceramics 11 as microphones, accelerometers, ultrasonic transducers, etc., were developed and commercialized in this period. Development of piezoceramic materials during and after World War II helped revolutionize this ﬁeld. During World War II, signiﬁcant research was performed in the United States and other countries such as Japan and the former Soviet Union which was aimed at the development of materials with very high dielectric constants for the construction of capacitors. Piezoceramic materials were discovered as a result of these activities, and a number of methods for their high-volume manufacturing were devised. The ability to build new piezoelectric devices by tailoring a material to a speciﬁc application resulted in a number of developments, and inventions such as: powerful sonars, piezo ignition systems, sensitive hydrophones and ceramic phono cartridges, to name a few. 2.3 Piezoelectric Ceramics A piezoelectric ceramic is a mass of perovskite crystals. Each crystal is composed of a small, tetravalent metal ion placed inside a lattice of larger divalent metal ions and O2 , as shown in Figure 2.1. To prepare a piezoelectric ceramic, ﬁne powders of the component metal oxides are mixed in speciﬁc proportions. This mixture is then heated to form a uniform powder. The powder is then mixed with an organic binder and is formed into speciﬁc shapes, e.g. discs, rods, plates, etc. These elements are then heated for a speciﬁc time, and under a predetermined temperature. As a result of this process the powder particles sinter and the material forms a dense crystalline structure. The elements are then cooled and, if needed, trimmed into speciﬁc shapes. Finally, electrodes are applied to the appropriate surfaces of the structure. Above a critical temperature, known as the “Curie temperature”, each perovskite crystal in the heated ceramic element exhibits a simple cubic symmetry with no dipole moment, as demonstrated in Figure 2.1. However, at temperatures below the Curie temperature each crystal has tetragonal symmetry and, associated with that, a dipole moment. Adjoining dipoles form regions of local alignment called “domains”. This alignment gives a net dipole moment to the domain, and thus a net polarization. As demonstrated in Figure 2.2 (a), the direction of polarization among neighboring domains is random. Subsequently, the ceramic element has no overall polarization. The domains in a ceramic element are aligned by exposing the element to a strong, DC electric ﬁeld, usually at a temperature slightly below the Curie temperature (Figure 2.2 (b)). This is referred to as the “poling process”. After the poling treatment, domains most nearly aligned with the electric ﬁeld expand at the expense of domains that are not aligned with the ﬁeld, and the element expands in the direction of the ﬁeld. When the electric ﬁeld is removed most of the dipoles are locked into a conﬁguration of near alignment 12 2 Fundamentals of Piezoelectricity Figure 2.1. Crystalline structure of a piezoelectric ceramic, before and after polarization (Figure 2.2 (c)). The element now has a permanent polarization, the remnant polarization, and is permanently elongated. The increase in the length of the element, however, is very small, usually within the micrometer range. Properties of a poled piezoelectric ceramic element can be explained by the series of images in Figure 2.3. Mechanical compression or tension on the element changes the dipole moment associated with that element. This creates a voltage. Compression along the direction of polarization, or tension perpendicular to the direction of polarization, generates voltage of the same polarity as the poling voltage (Figure 2.3 (b)). Tension along the direction of polarization, or compression perpendicular to that direction, generates a voltage with polarity opposite to that of the poling voltage (Figure 2.3 (c)). When operating in this mode, the device is being used as a sensor. That is, the ceramic element converts the mechanical energy of compression or tension into electrical energy. Values for compressive stress and the voltage (or ﬁeld Figure 2.2. Poling process: (a) Prior to polarization polar domains are oriented randomly; (b) A very large DC electric ﬁeld is used for polarization; (c) After the DC ﬁeld is removed, the remnant polarization remains. 2.4 Piezoelectric Constitutive Equations 13 Figure 2.3. Reaction of a poled piezoelectric element to applied stimuli strength) generated by applying stress to a piezoelectric ceramic element are linearly proportional, up to a speciﬁc stress, which depends on the material properties. The same is true for applied voltage and generated strain3 . If a voltage of the same polarity as the poling voltage is applied to a ceramic element, in the direction of the poling voltage, the element will lengthen and its diameter will become smaller (Figure 2.3 (d)). If a voltage of polarity opposite to that of the poling voltage is applied, the element will become shorter and broader (Figure 2.3 (e)). If an alternating voltage is applied to the device, the element will expand and contract cyclically, at the frequency of the applied voltage. When operated in this mode, the piezoelectric ceramic is used as an actuator. That is, electrical energy is converted into mechanical energy. 2.4 Piezoelectric Constitutive Equations In this section we introduce the equations which describe electromechanical properties of piezoelectric materials. The presentation is based on the IEEE standard for piezoelectricity [154] which is widely accepted as being a good representation of piezoelectric material properties. The IEEE standard assumes that piezoelectric materials are linear. It turns out that at low electric ﬁelds and at low mechanical stress levels piezoelectric materials have a linear proﬁle. However, they may show considerable nonlinearity if operated under a high electric ﬁeld or high mechanical stress level. In this book we are mainly concerned with the linear behavior of piezoelectric materials. That is, for the most part, we assume that the piezoelectric transducers are being operated at low electric ﬁeld levels and under low mechanical stress. When a poled piezoelectric ceramic is mechanically strained it becomes electrically polarized, producing an electric charge on the surface of the material. This property is referred to as the “direct piezoelectric eﬀect” and is the 3 It should be stressed that this statement is true when the piezoelectric material is being operated under small electric ﬁeld, or mechanical stress. When subject to higher mechanical, or electrical ﬁelds, piezoelectric transducers display hysteresistype nonlinearity. For the most part, in this monograph, the linear behavior of piezoelectric transducers will be of interest. However, Chapter 11 will brieﬂy review the issues arising when a piezoelectric transducer is operated in the nonlinear regime. 14 2 Fundamentals of Piezoelectricity z, 3 y, 2 x, 1 Piezoelectric Material + v − t Surface Electrodes Dipole Alignment Figure 2.4. Schematic diagram of a piezoelectric transducer basis upon which the piezoelectric materials are used as sensors. Furthermore, if electrodes are attached to the surfaces of the material, the generated electric charge can be collected and used. This property is particularly utilized in piezoelectric shunt damping applications to be discussed in Chapter 4. The constitutive equations describing the piezoelectric property are based on the assumption that the total strain in the transducer is the sum of mechanical strain induced by the mechanical stress and the controllable actuation strain caused by the applied electric voltage. The axes are identiﬁed by numerals rather than letters. In Figure 2.4, 1 refers to the x axis, 2 corresponds to the y axis, and 3 corresponds to the z axis. Axis 3 is assigned to the direction of the initial polarization of the piezoceramic, and axes 1 and 2 lie in the plane perpendicular to axis 3. This is demonstrated more clearly in Figure 2.5. The describing electromechanical equations for a linear piezoelectric material can be written as [154, 70]: E σj + dmi Em εi = Sij Dm = dmi σi + σ ξik Ek , (2.1) (2.2) where the indexes i, j = 1, 2, . . . , 6 and m, k = 1, 2, 3 refer to diﬀerent directions within the material coordinate system, as shown in Figure 2.5. The above equations can be re-written in the following form, which is often used for applications that involve sensing: D σj + gmi Dm εi = Sij σ Dk Ei = gmi σi + βik where (2.3) (2.4) 2.4 Piezoelectric Constitutive Equations z(3) P y(2) # – 1 2 3 4 5 6 15 Axis ——– x y z Shear around x Shear around y Shear around z x(1) Figure 2.5. Axis nomenclature σ ... ε ... E... ξ ... d ... S ... D. . . g ... β ... stress vector (N/m2 ) strain vector (m/m) vector of applied electric ﬁeld (V /m) permitivity (F/m) matrix of piezoelectric strain constants (m/V ) matrix of compliance coeﬃcients (m2 /N ) vector of electric displacement (C/m2 ) matrix of piezoelectric constants (m2 /C) impermitivity component (m/F ) Furthermore, the superscripts D, E, and σ represent measurements taken at constant electric displacement, constant electric ﬁeld and constant stress. Equations (2.1) and (2.3) express the converse piezoelectric eﬀect, which describe the situation when the device is being used as an actuator. Equations (2.2) and (2.4), on the other hand, express the direct piezoelectric eﬀect, which deals with the case when the transducer is being used as a sensor. The converse eﬀect is often used to determine the piezoelectric coeﬃcients. In matrix form, Equations (2.1)-(2.4) can be written as: ⎡ ⎤ ⎡ ε1 S11 ⎢ ε2 ⎥ ⎢S21 ⎢ ⎥ ⎢ ⎢ ε3 ⎥ ⎢S31 ⎢ ⎥=⎢ ⎢ ε4 ⎥ ⎢S41 ⎢ ⎥ ⎢ ⎣ ε5 ⎦ ⎣S51 ε6 S61 and ⎤⎡ ⎤ S12 S13 S14 S15 S16 σ1 ⎢ ⎥ S22 S23 S24 S25 S26 ⎥ ⎥ ⎢ σ2 ⎥ ⎥ ⎢ S32 S33 S34 S35 S36 ⎥ ⎢ σ3 ⎥ ⎥ ⎢ τ23 ⎥ S42 S43 S44 S45 S46 ⎥ ⎥⎢ ⎥ S52 S53 S54 S55 S56 ⎦ ⎣ τ31 ⎦ S62 S63 S64 S65 S66 τ12 ⎤ ⎡ d11 d21 d31 ⎢d12 d22 d32 ⎥ ⎡ ⎤ ⎥ ⎢ ⎢d13 d23 d33 ⎥ E1 ⎥⎣ ⎦ +⎢ ⎢d14 d24 d34 ⎥ E2 ⎥ ⎢ ⎣d15 d25 d35 ⎦ E3 d16 d26 d36 (2.5) 16 2 Fundamentals of Piezoelectricity ⎤ σ1 ⎡ ⎤ ⎡ ⎤ ⎢ σ2 ⎥ ⎥ D1 d11 d12 d13 d14 d15 d16 ⎢ ⎢ σ3 ⎥ ⎣ D2 ⎦ = ⎣d21 d22 d23 d24 d25 d26 ⎦ ⎢ ⎥ ⎢ σ4 ⎥ ⎥ D3 d31 d32 d33 d34 d35 d36 ⎢ ⎣ σ5 ⎦ σ6 ⎡ σ σ σ ⎤⎡ ⎤ e11 e12 e13 E1 σ σ σ + ⎣e21 e22 e23 ⎦ ⎣ E2 ⎦ . eσ31 eσ32 eσ33 E3 ⎡ (2.6) Some texts use the following notation for shear strain γ23 = ε4 γ31 = ε5 γ12 = ε6 and for shear stress τ23 = σ4 τ31 = σ5 τ12 = σ6 . Assuming that the device is poled along the axis 3, and viewing the piezoelectric material as a transversely isotropic material, which is true for piezoelectric ceramics, many of the parameters in the above matrices will be either zero, or can be expressed in terms of other parameters. In particular, the non-zero compliance coeﬃcients are: S11 = S22 S13 = S31 = S23 = S32 S12 = S21 S44 = S55 S66 = 2(S11 − S12 ). The non-zero piezoelectric strain constants are d31 = d32 and d15 = d24 . Finally, the non-zero dielectric coeﬃcients are eσ11 = eσ22 and eσ33 . Subsequently, the equations (2.5) and (2.6) are simpliﬁed to: 2.4 Piezoelectric Constitutive Equations ⎡ ⎤ ⎤⎡ σ1 S12 S13 0 0 0 ⎥ ⎢ σ2 ⎥ S11 S13 0 0 0 ⎥ ⎥⎢ ⎥ ⎢ σ3 ⎥ S13 S33 0 0 0 ⎥ ⎥⎢ ⎥ ⎢ τ23 ⎥ 0 0 S44 0 0 ⎥⎢ ⎥ ⎦ ⎣ τ31 ⎦ 0 0 0 0 S44 0 0 0 0 2(S11 − S12 ) τ12 ⎤ ⎡ 0 0 d31 ⎢ 0 0 d31 ⎥ ⎡ ⎤ ⎥ ⎢ ⎢ 0 0 d33 ⎥ E1 ⎥⎣ ⎦ +⎢ ⎢ 0 d15 0 ⎥ E2 ⎥ ⎢ ⎣d15 0 0 ⎦ E3 0 0 0 17 ⎤ ⎡ ε1 S11 ⎢ ε2 ⎥ ⎢S12 ⎢ ⎥ ⎢ ⎢ ε3 ⎥ ⎢S13 ⎢ ⎥=⎢ ⎢ ε4 ⎥ ⎢ 0 ⎢ ⎥ ⎢ ⎣ ε5 ⎦ ⎣ 0 0 ε6 (2.7) and ⎤ σ1 ⎡ ⎤ ⎢ σ2 ⎥ ⎤ ⎡ ⎥ D1 0 0 0 0 d15 0 ⎢ ⎢ σ3 ⎥ ⎣ D2 ⎦ = ⎣ 0 0 0 d15 0 0⎦ ⎢ ⎥ ⎢ σ4 ⎥ ⎥ d31 d31 d33 0 0 0 ⎢ D3 ⎣ σ5 ⎦ σ6 ⎡ σ ⎤⎡ ⎤ e11 0 0 E1 σ ⎣ ⎦ ⎣ + 0 e11 0 E2 ⎦ . σ E3 0 0 e33 ⎡ The “piezoelectric strain constant” d is deﬁned as the ratio of developed free strain to the applied electric ﬁeld. The subscript dij implies that the electric ﬁeld is applied or charge is collected in the i direction for a displacement or force in the j direction. The physical meaning of these, as well as other piezoelectric constants, will be explained in the following section. The actuation matrix in (2.5) applies to PZT materials. For actuators made of PVDF materials, this matrix should be modiﬁed to ⎤ ⎡ 0 0 d31 ⎢ 0 0 d32 ⎥ ⎢ ⎥ ⎢ 0 0 d33 ⎥ ⎥ ⎢ ⎢ 0 d25 0 ⎥ . ⎥ ⎢ ⎣d15 0 0 ⎦ 0 0 0 This reﬂects the fact that in PVDF ﬁlms the induced strain is nonisotropic on the surface of the ﬁlm. Hence, an electric ﬁeld applied in the direction of the polarization vector will result in diﬀerent strains in 1 and 2 directions. 18 2 Fundamentals of Piezoelectricity z(3) y(2) t V x(1) w Figure 2.6. A piezoelectric transducer arrangement for d31 measurement 2.5 Piezoelectric Coeﬃcients This section reviews the physical meaning of some of the piezoelectric coeﬃcients introduced in the previous section. Namely dij , gij , Sij and eij . 2.5.1 Piezoelectric Constant dij The piezoelectric coeﬃcient dij is the ratio of the strain in the j-axis to the electric ﬁeld applied along the i-axis, when all external stresses are held constant. In Figure 2.6, a voltage of V is applied to a piezoelectric transducer which is polarized in direction 3. This voltage generates the electric ﬁeld E3 = V t which strains the transducer. In particular ε1 = Δ in which d31 V . t The piezoelectric constant d31 is usually a negative number. This is due to the fact that application of a positive electric ﬁeld will generate a positive strain in direction 3. Another interpretation of dij is the ratio of short circuit charge per unit area ﬂowing between connected electrodes perpendicular to the j direction to the stress applied in the i direction. As shown in Figure 2.7, once a force F is applied to the transducer, in the 3 direction, it generates the stress Δ = σ3 = F w which results in the electric charge q = d33 F 2.5 Piezoelectric Coeﬃcients 19 F z(3) y(2) t x(1) SC w Figure 2.7. Charge deposition on a piezoelectric transducer - An equal, but opposite force, F , is not shown ﬂowing through the short circuit. If a stress is applied equally in 1, 2 and 3 directions, and the electrodes are perpendicular to axis 3, the resulting short-circuit charge (per unit area), divided by the applied stressed is denoted by dp . 2.5.2 Piezoelectric Constant gij The piezoelectric constant gij signiﬁes the electric ﬁeld developed along the i-axis when the material is stressed along the j-axis. Therefore, in Figure 2.8 the applied force F , results in the voltage V = g31 F . w Another interpretation of gij is the ratio of strain developed along the j-axis to the charge (per unit area) deposited on electrodes perpendicular to the i-axis. Therefore, in Figure 2.9, if an electric charge of Q is deposited on the surface electrodes, the thickness of the piezoelectric element will change by g31 Q Δ = . w F z(3) y(2) t + V − x(1) w Figure 2.8. An open-circuited piezoelectric transducer under a force in direction 1 - An equal, but opposite force, F , is not shown 20 2 Fundamentals of Piezoelectricity z(3) y(2) t x(1) q w Figure 2.9. A piezoelectric transducer subject to applied charge 2.5.3 Elastic Compliance Sij The elastic compliance constant Sij is the ratio of the strain the in i-direction to the stress in the j-direction, given that there is no change of stress along the other two directions. Direct strains and stresses are denoted by indices 1 to 3. Shear strains and stresses are denoted by indices 4 to 6. Subsequently, S12 signiﬁes the direct strain in the 1-axis when the device is stressed along the 2-axis, and stresses along directions 1 and 3 are unchanged. Similarly, S44 refers to the shear strain around the 2-axis due to the shear stress around the same axis. E is meaA superscript “E” is used to state that the elastic compliance Sij sured with the electrodes short-circuited. Similarly, the superscript “D” in D denotes that the measurements were taken when the electrodes were left Sij open-circuited. A mechanical stress results in an electrical response that can E to be smaller increase the resultant strain. Therefore, it is natural to expect Sij D than Sij . That is, a short-circuited piezo has a smaller Young’s modulus of elasticity than when it is open-circuited. 2.5.4 Dielectric Coeﬃcient, eij The dielectric coeﬃcient eij determines the charge per unit area in the i-axis due to an electric ﬁeld applied in the j-axis. In most piezoelectric materials, a ﬁeld applied along the j-axis causes electric displacement only in that direction. The relative dielectric constant, deﬁned as the ratio of the absolute permitivity of the material by permitivity of free space, is denoted by K. The superscript σ in eσ11 refers to the permitivity for a ﬁeld applied in the 1 direction, when the material is not restrained. 2.5.5 Piezoelectric Coupling Coeﬃcient kij The piezoelectric coeﬃcient kij represents the ability of a piezoceramic material to transform electrical energy to mechanical energy and vice versa. This transformation of energy between mechanical and electrical domains is employed in both sensors and actuators made from piezoelectric materials. The 2.5 Piezoelectric Coeﬃcients 21 ij index indicates that the stress, or strain is in the direction j, and the electrodes are perpendicular to the i-axis. For example, if a piezoceramic is mechanically strained in direction 1, as a result of electrical energy input in direction 3, while the device is under no external stress, then the ratio of 2 . stored mechanical energy to the applied electrical energy is denoted as k31 There are a number of ways that kij can be measured. One possibility is to apply a force to the piezoelectric element, while leaving its terminals open-circuited. The piezoelectric device will deﬂect, similar to a spring. This deﬂection Δz , can be measured and the mechanical work done by the applied force F can be determined F Δz WM = . 2 Due to the piezoelectric eﬀect, electric charges will be accumulated on the transducer’s electrodes. This amounts to the electrical energy Q2 WE = 2Cp which is stored in the piezoelectric capacitor. Therefore, WE k33 = WM Q = . F Δz Cp The coupling coeﬃcient can be written in terms of other piezoelectric constants. In particular 2 kij = d2ij E eσ Sij ij = gij dij Ep , (2.8) where Ep is the Young’s modulus of elasticity of the piezoelectric material. When a force is applied to a piezoelectric transducer, depending on whether the device is open-circuited or short-circuited, one should expect to observe diﬀerent stiﬀnesses. In particular, if the electrodes are short-circuited, the device will appear to be “less stiﬀ”. This is due to the fact that upon the application of a force, the electric charges of opposite polarities accumulated on the electrodes cancel each other. Subsequently no electrical energy can be stored in the piezoelectric capacitor. Denoting short-circuit stiﬀness and open-circuit stiﬀness respectively as Ksc and Koc , it can be proved that Koc 1 = . Ksc 1 − k2 22 2 Fundamentals of Piezoelectricity 2.6 Piezoelectric Sensor When a piezoelectric transducer is mechanically stressed, it generates a voltage. This phenomenon is governed by the direct piezoelectric eﬀect (2.2). This property makes piezoelectric transducers suitable for sensing applications. Compared to strain gauges, piezoelectric sensors oﬀer superior signal to noise ratio, and better high-frequency noise rejection. Piezoelectric sensors are, therefore, quite suitable for applications that involve measuring low strain levels. They are compact, easy to embed and require moderate signal conditioning circuitry. If a PZT sensor is subject to a stress ﬁeld, assuming the applied electric ﬁeld is zero, the resulting electrical displacement vector is: ⎧ ⎫ σ1 ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎫ ⎡ ⎧ ⎤⎪ σ ⎪ ⎪ 2 ⎪ ⎪ 0 0 0 0 d15 0 ⎨ ⎬ ⎨ D1 ⎬ σ 3 ⎦ ⎣ D2 = 0 0 0 d15 0 0 . ⎪ τ23 ⎪ ⎭ ⎩ ⎪ d31 d31 d33 0 0 0 ⎪ D3 ⎪ ⎪ ⎪ τ31 ⎪ ⎪ ⎪ ⎪ ⎪ ⎭ ⎩ τ12 The generated charge can be determined from ⎤ ⎡ dA 1 D1 D2 D3 ⎣dA2 ⎦ , q= dA3 where dA1 , dA2 and dA3 are, respectively, the diﬀerential electrode areas in the 2-3, 1-3 and 1-2 planes. The generated voltage Vp is related to the charge via q , Vp = Cp where Cp is capacitance of the piezoelectric sensor. Having measured the voltage, Vp , strain can be determined by solving the above integral. If the sensor is a PZT patch with two faces coated with thin electrode layers, e.g. the patch in Figure 2.4, and if the stress ﬁeld only exists along the 1-axis, the capacitance can be determined from weσ33 . Cp = t Assuming the resulting strain is along the 1-axis, the sensor voltage is found to be d31 Ep w Vs = ε1 dx, (2.9) Cp where Ep is the Young’s modulus of the sensor and ε1 is averaged over the sensor’s length. The strain can then be calculated from 2.7 Piezoelectric Actuator ε1 = Cp Vs . d31 Ep w 23 (2.10) In deriving the above equation, the main assumption was that the sensor was strained only along 1-axis. If this assumption is violated, which is often the case, then (2.10) should be modiﬁed to ε1 = Cp Vs , (1 − ν)d31 Ep w where ν is the Poisson’s ratio4 . 2.7 Piezoelectric Actuator Consider a beam with a pair of collocated piezoelectric transducers bonded to it as shown in Figure 2.10. The purpose of actuators is to generate bending in the beam by applying a moment to it. This is done by applying equal voltages, of 180◦ phase diﬀerence, to the two patches. Therefore, when one patch expands, the other contracts. Due to the phase diﬀerence between the voltages applied to the two actuators, only pure bending of the beam will occur, without any excitation of longitudinal waves. The analysis presented in this section follows the research reported in references [42, 11, 76, 53]. When a voltage V is applied to one of the piezoelectric elements, in the direction of the polarization vector, the actuator strains in direction 1 (the x-axis). Furthermore, the amount of free strain is given by εp = d31 V , tp (2.11) where tp represents the thickness of the piezoelectric actuator. Since the piezoelectric patch is bonded to the beam, its movements are constrained by the stiﬀness of the beam. In the foregoing analysis perfect bonding of the actuator to the beam is assumed. In other words, the shearing eﬀect of the non-ideal bonding layer is ignored [33]. Assuming that the strain distribution is linear across the thickness of the beam5 , we may write ε(z) = αz. (2.12) The above equation represents the strain distribution throughout the beam, and the piezoelectric patches, if the composite structure were bent, say by an external load, into a downward curvature. Subsequently, the portion of the beam above the neutral axis and the top patch would be placed in 4 5 Notice that if d31 = d32 , e.g. if the sensor is a PVDF ﬁlm, then this expression Cp Vs . for strain must be changed to ε1 = d32 (1−ν d 31 )d31 Ep w This is consistent with the Kirchoﬀ hypothesis of laminate plate theory[97]. 24 2 Fundamentals of Piezoelectricity Figure 2.10. A beam with a pair of identical collocated piezoelectric actuators tension, and the bottom half of the structure and the bottom patch in compression. Although, the strain is continuous on the beam-actuator surface, the stress distribution is discontinuous. In particular, using Hooke’s law, the stress distribution within the beam is found to be σb (z) = Eb αz, (2.13) where Eb is the Young’s modulus of elasticity of the beam. Since the two “identical” piezoelectric actuators are constrained by the beam, stress distributions inside the top and the bottom actuators can be written in terms of the total strain in each actuator (the strain that produces stress) σpt = Ep (αz − εp ) (2.14) σpb = Ep (αz + εp ), (2.15) where Ep is the Young’s modulus of elasticity of the piezoelectric material and the superscripts t and b refer to the top and bottom piezoelectric patches respectively. Applying moment equilibrium about the center of the beam6 results in − tb 2 t − 2b −tp σpb (z)zdz + tb 2 t − 2b σp (z)zdz + tb 2 tb 2 +tp σpt (z)zdz = 0. After integration α is determined to be 3Ep ( t2b + tp )2 − ( t2b )2 εp . α = tb 2 Ep ( 2 + tp )3 − ( t2b )3 + Eb ( t2b )3 6 (2.16) (2.17) Due to the symmetrical nature of the stress ﬁeld, the integration need only tb be carried out starting from the centre of the beam, i.e. 0 2 σp (z)zdz + t2b +tp t σp (z)zdz = 0. tb 2 2.7 Piezoelectric Actuator 25 Figure 2.11. A beam with a single piezoelectric actuator The induced moment intensity7 , M in the beam is then determined by integrating the triangular stress distribution across the beam: M = Eb Iα, (2.18) where I is the beam’s moment of inertia. Knowledge of M is crucial in determining the dynamics of the piezoelectric laminate beam. If only one piezoelectric actuator is bonded to the beam, such as shown in Figure 2.11, then the strain distribution (2.12) needs to be modiﬁed to ε(z) = (αz + ε0 ). (2.19) This expression for strain distribution across the beam thickness can be decomposed into two parts: the ﬂexural component, αz and the longitudinal component, ε0 . Therefore, the beam extends and bends at the same time. This is demonstrated in Figure 2.12. The stress distribution inside the piezoelectric actuator is found to be σp (z) = Ep (αz + ε0 − εp ). (2.20) The two parameters, ε0 and α can be determined by applying the moment equilibrium about the centre of the beam Figure 2.12. Decomposition of asymmetric stress distribution (a) into two parts: (b) ﬂexural and (c) longitudinal components. 7 moment per unit length 26 2 Fundamentals of Piezoelectricity tb 2 − tb 2 σb (z)zdz + tb 2 +tp tb 2 σp (z)zdz = 0 (2.21) σp (z)dz = 0. (2.22) and the force equilibrium along the x-axis tb 2 − tb 2 σb (z)dz + tb 2 +tp tb 2 Unlike the symmetric case, the force equilibrium condition (2.22) needs to be applied. This is due to the asymmetric distribution of strain throughout the beam. Solving (2.21) and (2.22) for ε0 and α we obtain α= and Eb2 t4b 6Eb Ep tb tp (tb + tp ) εp + Ep Eb (4t3b tp + 6t2b t2p + 4tb t3p ) + Ep2 tp {Eb t3p + Ep t3p }Ep (tb /2) ε0 = 2 4 εp . Eb tb + Ep Eb (4t3b tp + 6t2b t2p + 4tb t3p ) + Ep2 tp (2.23) (2.24) The response of the beam to this form of actuation consists of a moment distribution Mx = Eb Iα (2.25) and a longitudinal strain distribution εx = ε0 . (2.26) It can be observed that the moment exerted on the beam by one actuator is not exactly half of that applied by two collocated piezoelectric actuators driven by 180◦ out-of-phase voltages. This arises from the fact that the Expressions (2.25) and (2.23) do not include the eﬀect of the second piezoelectric actuator. However, if this eﬀect is included by allowing for the stiﬀness of the second actuator in the derivations, while ensuring that the voltage applied to this patch is set to zero, then it can be shown that the resulting moment will be exactly half of that predicted by (2.18) and (2.17). The collocated situation is often used in vibration control applications, in which one piezoelectric transducer is used as an actuator while the other one is used as a sensor. This conﬁguration is appealing for feedback control applications for reasons that will be explained in Chapter 3. 2.8 Piezoelectric 2D Actuation This section is concerned with the use of piezoelectric actuators for excitation of two-dimensional structures, such as plates in pure bending. The analysis is similar to that presented in the previous section. A typical application is 2.8 Piezoelectric 2D Actuation z 27 y x Figure 2.13. A piezoelectric actuator bonded to a plate shown in Figure 2.13, which demonstrates a piezoelectric transducer bonded to the surface of a plate. It is also assumed that another identical transducer is bonded to the opposite side of the structure in a collocated fashion. If the two patches are driven by signals that are 180◦ out of phase, the resulting strain distribution, across the plate, will be linear as shown in Figure 2.14 a and b. That is, εx = αx z εy = αy z, (2.27) (2.28) where αx and αy represent the strain distribution slopes in the x − z and y − z planes respectively. Assuming that the piezoelectric material has similar properties in the 1 and 2 directions, i.e. d31 = d32 , the unconstrained strain associated with the actuator in both the x and y directions, under the voltage V , is given by εp = d31 V . tp Now the resulting stresses in the plate, in the x and y directions are σx = and E (εx + νεy ) 1 − ν2 E (εy + νεx ), 1 − ν2 where ν is the Poisson’s ratio of the plate material. Representing the stresses in the top piezoelectric patch as σxp and σyp , and the stresses in the bottom patch as σ̃xp and σ̃yp , we may write σy = 28 2 Fundamentals of Piezoelectricity z x x (a) z y y (b) Figure 2.14. Two dimensional strain distribution in a plane with two collocated anti-symmetric piezoelectric actuators Ep 1 − νp2 Ep σ̃xp = 1 − νp2 Ep σyp = 1 − νp2 Ep σ̃yp = 1 − νp2 σxp = {εx + νp εy − (1 + νp )εp } (2.29) {εx + νp εy + (1 + νp )εp } (2.30) {εy + νp εx − (1 + νp )εp } (2.31) {εy + νp εx + (1 + νp )εp } , (2.32) where νp is the Poisson’s ratio of the piezoelectric material. Given that εp is the same in both directions and that the plate is homogeneous, we may write εx = εy = ε. Subsequently, the strain distribution across the plate thickness can be written as ε = αx z = αy z = αz. 2.9 Dynamics of a Piezoelectric Laminate Beam 29 The condition of moment of equilibrium about the x and y axes can now be applied. That is, 2t 2t +tp σx zdz + σxp zdz = 0 0 and 0 t 2 t 2 σy zdz + t 2 +tp t 2 σyp zdz = 0, where t represents the plate’s thickness. Integrating and solving for α gives α= 2Ep {( t2b 3Ep {( t2b + tp )2 − ( t2b )2 }(1 − ν) εp . + tp )3 − ( t2b )3 }(1 − ν) + 2E( t2b )3 (1 − νp ) The resulting moments in x and y directions are Mx = My = EIα. (2.33) For the symmetric case, i.e. when only one piezoelectric actuator is bonded to the plate, similar derivations to the previous section can be made. 2.9 Dynamics of a Piezoelectric Laminate Beam In this section we explain how the dynamics of a beam with a number of collocated piezoelectric actuator/sensor pairs can be derived. At this stage we do not make any speciﬁc assumptions about the boundary conditions since we wish to keep the discussion as general as possible. However, we will explain how the eﬀect of boundary conditions can be incorporated into the model. Let us consider a setup as shown in Figure 2.15, where m identical collocated piezoelectric actuator/sensor pairs are bonded to a beam. The assumption that all piezoelectric transducers are identical is only adopted to simplify the derivations, and can be removed if necessary. The ith actuator is exposed to a voltage of vai (t) and the voltage induced in the ith sensor is vpi (t). We assume that the beam has a length of L, width of W , and thickness of tb . Corresponding dimensions of each piezoelectric transducer are Lp , Wp , and tp . Furthermore, we denote the transverse deﬂection of the beam at point x and time t by z(x, t). The dynamics of such a structure are governed by the Bernoulli-Euler partial diﬀerential equation ∂ 2 z(x, t) ∂ 4 z(x, t) ∂ 2 Mx (x, t) + ρA = , (2.34) b ∂x4 ∂t2 ∂x2 where ρ, Ab , Eb and I represent density, cross-sectional area, Young’s modulus of elasticity and moment of inertia about the neutral axis of the beam respectively. The total moment acting on the beam is represented by Mx (x, t), which is the sum of moments exerted on the beam by each actuator, i.e. Eb I 30 2 Fundamentals of Piezoelectricity x2i x1i tp ... ... Actuators ... ... Sensors tb /2 Figure 2.15. A beam with a number of collocated piezoelectric actuator/sensor pairs Mx (x, t) = m Mxi (x, t). (2.35) i=1 The moment exerted on the beam by the ith actuator, Mxi (x, t) can be written as Mxi (x, t) = κ̄vai (t){u(x − x1i ) − u(x − x2i )}, (2.36) where u(x) represents the unit step function, i.e. u(x) = 0 for x < 0 and u(x) = 1 for x ≥ 0. The term {u(x − x1i ) − u(x − x2i )} is incorporated into (2.36) to account for the spatial placement of the ith actuator. The constant κ̄ can be determined from (2.11), (2.17) and (2.18). The forcing term in (2.34) can now be determined from Expressions (2.36) and (2.35), and using the following property of Dirac delta function ∞ δ (n) (t − θ)φ(t)dt = (−1)n φ(n) (θ), (2.37) −∞ where δ (n) is the nth derivative of δ, and φ is a continuous function of θ [111]. Having determined the expression for the forcing function in (2.34) we can now proceed to solving the partial diﬀerential equation. One approach to solving this PDE is based on using the modal analysis approach [130]. In this technique the solution of the PDE is assumed to be of the form z(x, t) = ∞ wk (x)qk (t). (2.38) k=1 Here wk (x), known as the modeshape, is the eigenfunction which is determined from the eigenvalue problem obtained by substituting (2.38) into (2.34) and using the following orthogonality properties [130] L wk (x)wp (x)dx = δkp (2.39) 0 L 0 Eb I d4 wk (x) wp (x)dx = ωk2 δkp , ρAb dx4 (2.40) 2.9 Dynamics of a Piezoelectric Laminate Beam 31 where ωk describes the k th natural frequency of the beam and δkp is the Kroneker delta function, i.e. 1, k = p δkp = 0, otherwise A solution to the eigenvalue problem requires precise knowledge of boundary conditions. For speciﬁc boundary conditions, e.g. simply-supported and cantilevered, mode shapes and resonance frequencies can be determined analytically from the eigenvalue problem. For further details, the reader is referred to [130] and [50]. A set of uncoupled ordinary diﬀerential equations can be obtained from (2.34) using the orthogonality properties (2.39) and (2.40) and the property (2.37), as well as (2.38). It can be shown that the ordinary diﬀerential equations are of the form: q̈k (t) + ωk2 qk (t) m κ̄ = ψk va (t), ρAb i=1 i i (2.41) where k = 1, 2, . . . and qk (t) is the generalized coordinate of the k th mode. Furthermore, the parameter ψki is found to be: ψki = = L wk (x) {δ (x − x1i ) − δ (x − x2i )} dx 0 wk (x2i ) − wk (x1i ), (2.42) (2.43) where f (x) represents the ﬁrst derivative of the function f with respect to x, and we have used (2.37) to obtain (2.43) from (2.42). To this end we point out that the diﬀerential equation (2.41) does not contain a term to account for the natural damping associated with the beam. The presence of damping can be incorporated into (2.41) by adding the term 2ζk q̇k (t) to (2.41). This results in the diﬀerential equation q̈k (t) + 2ζk ωk q̇k (t) + ωk2 qk (t) m κ̄ = ψk va (t). ρAb i=1 i i (2.44) Applying the Laplace transform to (2.44), assuming zero initial conditions, we obtain the following transfer function from the vector of applied actuator voltages Va (s) = [va1 (s), . . . , vam (s)] to the beam deﬂection z(x, s) at location x G(x, s) = γ ∞ i=1 where γ = κ̄ ρAb and wk (x)ψ̄k , s2 + 2ζk ωk s + ωk2 (2.45) 32 2 Fundamentals of Piezoelectricity ⎡ ⎤ ψk1 ⎢ ⎥ ψ̄k = ⎣ ... ⎦ . ψkm The piezoelectric voltage induced in the ith sensor can be obtained using Expression (2.9). That is, d31 Ep Wp vpi (t) = Cp 0 L εxi dx. The expression for the mechanical strain in the ith sensor patch can be obtained from 2 tb ∂ z εxi = − + tp . 2 ∂x2 Now vpi is found to be ∞ −d31 Ep Wp t2b + tp vpi (t) = ψki qk (t). Cp (2.46) k=1 Therefore, the transfer function matrix relating the voltages applied to the piezoelectric actuators Va (s) = [va1 (s), . . . , vam (s)] to the voltages measured at the piezoelectric sensors Vp (s) = [vp1 (s), . . . , vpm (s)] is found to be: Gvv (s) = γ̄ ∞ k=1 where ψ̄k ψ̄k , s2 + 2ζk ωk s + ωk2 (2.47) −d31 Ep Wp t2b + tp κ̄ . γ̄ = Cp ρAb To this end we need to explain how the systems represented by Inﬁnite Series (2.47) and (2.45) can be approximated with ﬁnite dimensional models. In any controller design scenario we may only be interested in designing a controller for a ﬁnite bandwidth. If N modes of the structure lie within that bandwidth of interest, the series (2.47) and (2.45) are often truncated to obtain a ﬁnite dimensional model of the structure, which is of minimum dimensions. While the truncation may not be of concern in non-collocated models, e.g. (2.45), it can be a serious problem for a collocated system, e.g. (2.47). Truncation of a collocated model can result in perturbations in open-loop zeros of the system, which in the worst case can cause closed-loop instabilities, and in the best case will contribute to the loss of closed-loop performance [34]. A number of techniques have been proposed to compensate for the effect of truncated out-of-bandwidth modes on collocated structural models. The reader is referred to [34, 207, 138, 135, 84] and references therein for an overview of such techniques. We do, however, point out that the truncation 2.10 Active and Macro Fiber Composite Transducers 33 w P w P + i + C p + v vs − − vs − SENSOR vp Cp + + −vp − − + v − ACTUATOR (a) (b) Figure 2.16. (a) A ﬂexible structure with a pair of collocated piezoelectric transducers, and (b) its electrical equivalent model error can be minimized by appending the truncated model by a feed-through term, i.e. to approximate (2.47) with Gvv (s) = γ̄ N k=1 ψ̄k ψ̄k + D. s2 + 2ζk ωk s + ωk2 If chosen properly, the addition of this feed-through term to the truncated model can result in an acceptable approximation. In this book, in most cases, we will use system identiﬁcation to directly identify this parameter, as well as the rest of the dynamics of the system. We conclude this chapter with an important observation that will be utilized in the forthcoming chapters. Figure 2.16 (a) illustrates a ﬂexible structure with a collocated piezoelectric actuator/sensor pair. The piezoelectric transducer on the right functions as an actuator, and the one on the left as a sensor. What is of importance here is the electrical model of the system depicted in Figure 2.16 (b). Each piezoelectric transducer is modeled as a capacitor in series with a strain-dependent voltage source. The transfer function from the voltage applied to the actuator, v to the voltage induced in the sensor, vs = vp is given by (2.47). This observation is particularly important in designing piezoelectric shunts, and to identify the connection between piezoelectric shunt damping and feedback control of a collocated system. This will be discussed in more detail in Chapter 5. 2.10 Active and Macro Fiber Composite Transducers Active Fiber Composites (AFCs) are an alternative to traditional monolithic piezoelectric transducers. First proposed in 1992 [20], longitudinally polarized 34 2 Fundamentals of Piezoelectricity + Figure 2.17. A piezoelectric Active Fiber Composite (AFC) comprised of piezoelectric ﬁbers with interdigitated electrodes top and bottom piezoelectric ﬁbers, as shown in Figure 2.17, are encased in an epoxy resin with interdigitated electrodes laminated onto the top and bottom surfaces of the transducer. With an applied voltage, the interdigitated electrodes induce longitudinal electric ﬁelds along the length of each ﬁber. The original motivation was to increase the electromechanical coupling by utilizing the high d33 piezoelectric strain constant rather than the lesser d31 constant. Active ﬁber composites have a number of practical advantages over traditional monolithic transducers [19]: • • • • The ﬁbers are encapsulated by the printed polymer electrodes and epoxy resin thus increasing the reliability and service-life in harsh environments. The short length and diameter or the ﬁbers together with their alignment along the length of the transducer increases the conformability of AFC transducers. They can be laminated onto structures with complex geometries and curvatures. AFC transducers are more robust to mechanical failure than monolithic transducers. In addition to their conformability, they can also tolerate local and incremental damage. If some of the ﬁbers are fractured, the transducer will not be substantially damaged, in contrast, monolithic actuators will fracture and fail if they are stressed beyond their yield limit. AFCs have been reported to develop greater strains than monolithic actuators [19]. The strain actuation is also unidirectional. Macro Fiber Composites (MFCs) [174] are similar in nature to AFCs as they utilize the direct d33 piezoelectric eﬀect through the use of interdigitated electrodes. Rather than individual ﬁbers, a monolithic transducer is simply cut into a number of long strips. The resulting transducer is conformable in one dimension and more robust to mechanical failure than monolithic patches. The greatest disadvantages of AFC and MFC transducers is their high present cost, and the large voltages required to achieve the same actuation strain as monolithic transducers. The equivalent piezoelectric capacitance is also much lesser making them unsuitable as low-frequency strain sensors (see Section 6.2). 2.10 Active and Macro Fiber Composite Transducers 35 The low capacitance of AFC and MFC transducers also causes diﬃculties in the implementation of piezoelectric shunt damping systems, to be discussed in Chapter 4. Device capacitances of less than 50 nF have been deemed impractical for shunt damping [18]. A performance comparison of monolithic, AFC, and MFC transducers in a passive shunt damping application can be found in references [18] and [148]. Although the piezoelectric transducers used throughout this book are exclusively monolithic, all of the techniques discussed in the proceeding chapters are equally as applicable to AFC and MFC variants. Indeed, from the control engineers viewpoint, transducer physics is usually lumped into a simpliﬁed electrical model, or identiﬁed as part of the structural system.